Facets of Lyotropic Liquid Crystals L. Latypova,† W. T. Gózd́ ź,*,† and P. Pierański‡ †

Institute of Physical Chemistry , Polish Academy of Sciences, Kasprzaka 44/52, 01-224 Warsaw, Poland Laboratoire de Physique des Solides, Université Paris-Sud, Bât. 510, 91405 Orsay, Cedex, France

‡

S Supporting Information *

ABSTRACT: The bicontinuous lyotropic liquid phases surrounded by the isotropic phase form monocrystals with well-developed facets. We investigate the structure and stability of the facets formed by the bicontinuous phase of Pn3̅m symmetry, at three preferred directions, which are developed on a spherical droplet of Pn3̅m phase surrounded by the isotropic phase. The structure of the facets is obtained by minimization of the Landau−Brazovskii functional with one scalar order parameter. for example the monocrystals of cubic phases12 or dispersion of nanoparticles built of cubic phases in the isotropic phase.13−16 Such nanoparticles are called cubosomes and may be used as nanocontainers for drug delivery, in a similar way as liposomes. When the bicontinuous phase coexists with an isotropic phase, its structure at the interface has to be deformed in order to avoid free edges of the bilayer exposed to the isotropic phase because the free edges are mainly built of hydrocarbon chains. Because of the hydrophobic eﬀect, the free edges connect with each other and the bilayer in the bicontinuous phase forms a closed surface, where the surface is deﬁned by the midplane of the bilayer. It is obvious that it is not possible to close the channels of the triply periodic surface with a zero mean curvature surface. The surface at the interface has to be built of the pieces of the surface with positive and negative mean curvatures. This will result in an increase of the bending energy (eq 1). The bending energy increase depends on the direction of the interface with respect to the unit cell, since the periodic bicontinuous phase is not isotropic. Unfortunately, the structure of the interface between the bicontinuous and the isotropic phases cannot be directly observed experimentally. The measurements of the surface tension for such interfaces were not yet conducted. The question of the shape and elastic energy of the surface representing the lipid bilayer at the interface between the cubic and isotropic phases remains open. It is the subject of the present study. Most of the work devoted to the studies of nanoparticles and monocrystals of the cubic lyotropic liquid crystal is experimental.12,14−16 It has been observed in experiments17 that the formation of facets on a spherical droplet of the bicontinuous lyotropic liquid phase of symmetry Pn3̅m takes place in a well-deﬁned order. First, the facet (111) is created next (100) and (110) (see Figure 1). The order of facets formation must be related to their stability, and the stability

1. INTRODUCTION Bicontinuous cubic lyotropic phases are ones of the most fascinating in nature. They are liquids with crystalline order, periodicity in x, y, and z directions having the length scale much larger than the size of molecules. They are formed in systems with competing interactions,1,2 such as diblock copolymers, ternary mixtures of oil, water and surfactants, or binary mixtures of lipids and water,3−6 and they can be encountered in biological cells in endoplasmic reticulum and organella.7 In this work, we focus on bicontinuous phases in mixtures of lipids and water. The amphiphilic lipid molecules self-assemble into a bilayer with the hydrocarbon chains isolated from the water molecules. The bilayer divides the volume into two disjoint networks of channels ﬁlled with water and behaves as an elastic membrane. For a ﬁxed topology, the elastic energy of the membrane depends on the mean curvature, H, of the surface describing the center of the bilayer according to the Helfrich formula:8 Fb = 2κ

∫ H 2 dA

(1)

where κ is the bending rigidity and dA is the inﬁnitesimal area element. Formula 1 may be applied for the systems with ﬁxed topology where according to Gauss−Bonnet theorem the surface integral of the Gaussian curvature is constant. In equilibrium the elastic energy assumes the minimum. In the bulk, the minimum of (1) corresponds to triply periodic minimal surface because the minimal surfaces have zero mean curvature at every point. The surface with zero mean curvature has saddle-like shape at every point (except ﬂat points). A plane is a special case of the minimal surface. The functional (1) has been successfully applied to the studies of vesicles built of lipid bilayers. The agreement between experimental results and the calculations performed for diﬀerent shapes of vesicles was excellent.9−11 In physical systems triply periodic surfaces cannot extend to inﬁnity. They have to be bounded by the walls of the vessel or by the surrounding coexisting phases. The latter case concerns © 2013 American Chemical Society

Received: October 22, 2013 Revised: December 28, 2013 Published: December 29, 2013 488

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

Figure 1. Phase transition L2 + Pn3m ̅ + L1 → Pn3m ̅ + L1 obtained by decreasing the concentration of ethanol in the L1 phase from 12% to 8% at constant temperature T = 43 °C, in the three-component mixture of water, ethanol, and phytantriol.17 L1 is the direct micellar phase, and L2 is the inverted micellar phase.

must be related to the structure of the facets, because diﬀerent curvatures of the surfaces closing the free edges result in diﬀerent values of the energy (eq 1). However, it is diﬃcult to determine experimentally the structure of the facets of monocrystals of lyotropic bicontinuous phases. The size of the unit cell of the cubic bicontinuous phases is much smaller than the resolution of the optical microscopes. Since the monocrystals are soft, application of AFM (atomic force microscopy) techniques is also problematic. Cryo-TEM (transmission electron microscopy) methods are the most useful so far. Unfortunately, the images obtained from cryoTEM experiments are generated by electrons scattered through the whole sample. Thus, limited information about the structure of the surface of the sample can be inferred indirectly from cryo-TEM experiments. The knowledge about the structure of the surface of the cubosomes and monocrystals could be obtained from appropriate theoretical calculations. So far, however, the theoretical description is restricted to purely geometrical models based on the properties of triply periodic nodal surfaces18 and to lattice models.19−21 The mathematical modeling based on the nodal surfaces allows for investigation of topological properties of the studied structures, but the shape of the bilayer and the elastic energy (1) of the examined object cannot be determined. Therefore, it is necessary to use appropriate free energy models to obtain the knowledge on the shape and the excess energy of the bilayer at the interface with an isotropic phase. The surface tension for the (111) and (100) orientations for the bicontinuous phase conﬁned by the hydrophilic walls was calculated in refs 19 and 20 in the lattice model for diﬀerent thickness of the slits. However, the surface tension in lattice models depends on the orientation of the interface with respect to the principal lattice directions even in the case of gas−liquid coexistence. For this reason it was not possible to compare the surface energies for diﬀerent orientations of the cubic phase with respect to the slit walls19 or an interface. Morover, in the lattice model from ref 21 only a few lattice points form a cubic cell. Therefore, the detailed structure of the bicontinuous phase at the wall cannot be determined. We are interested in the geometry and stability of interfaces formed when the Pn3̅m phase is surrounded by an isotropic phase. In particular, we would like to examine the geometry of the facets formed at the droplet of the Pn3̅m phase. The mathematical modeling of the bicontinuous phases in terms of the functional (1) is however very diﬃcult in the presence of the interface. It requires minimization of the functional (1) for functions describing the location of the bilayer. These functions are not know a priori and cannot be easily parametrized. Therefore, we decided to perform the calculations within the framework of a relatively simple Landau−Brazovskii type model

with one scalar order parameter related to the local concentration of water.22,23 In section 2 the functional and the computational method are described. In section 3 we present the results for the structure and related excess energy of the facets. In section 4 we show the experimental results for monocrystals and cubosomes.

2. THE MODEL AND THE COMPUTATIONAL METHOD The Landau−Brazovskii Type Functional. The freeenergy functional for systems inhomogeneous on the mesoscopic length scale can be written in the form -[ϕ(r)] =

∫ d3r(|Δϕ(r)|2 + g[ϕ(r)]|∇ϕ(r)|2 + f [ϕ(r)]) (2)

This functional successfully describes systems as diverse as binary or ternary surfactant mixtures, block copolymers, colloidal particles with competing attractive and repulsive interactions of diﬀerent range, or magnetic systems with competing ferromagnetic and antiferromagnetic interactions.1,2,22,24−27 The order parameter ϕ(r) in eq 2 depends on the physical context. In the case of block copolymers or ternary water−surfactant−oil mixtures ϕ(r) is the local concentration diﬀerence between the polar and the nonpolar components. In the case of lipids in water ϕ2(r) describes the local concentration of water. At the center of the lipid bilayer ϕ(r) = 0. The bilayer divides the space into two disjoint water channels: one of them on one side of the bilayer, where ϕ(r) > 0, and the other one on the other side of the bilayer, where ϕ(r) < 0. The sign of ϕ(r) allows to distinguish between the two disjoint channels of water. The ﬂuid in each channel, however, has the same physical nature. For this reason in the case of lipids in water the functional (2) must be an even function of ϕ. In homogeneous phases the concentration of water is independent of the position. In such a case ϕ(r) = const and ∇ϕ = Δϕ = 0, therefore f [ϕ] is the free-energy density of the homogeneous phases. In the case of the phase coexistence between water- and lipid-rich phases, we can postulate for f [ϕ] the form with three minima of equal depth, where ϕ = ±1 both represent the water-rich phase, f [ϕ(r)] = (ϕ(r)2 − 1)2(ϕ(r))2. The inhomogeneous distribution of the components, in particular the formation of the bilayer, is possible when the corresponding free energy is lower than for any homogeneous structure. When the concentration ϕ(r) becomes positiondependent, then (∇ϕ)2 > 0. - can decrease for (∇ϕ)2 increasing from 0 when g[ϕ(r)] < 0. On the other hand, the Laplacian term |Δϕ|2 leads to the increase of - , and the length scale of the inhomogeneities (the size of the unit cell in the case of the periodic phases) is determined by the competition between the terms supporting and suppressing the spatial 489

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

⎛ 2π ⎞ ⎛ 2π ⎞ ψD(x1 , x 2 , x3) = cos⎜ x1⎟ cos⎜ x 2⎟ ⎝L ⎠ ⎝L ⎠

oscillations of ϕ(r). Unlike in refs 1, 2, and 25−27 where g[ϕ(r)] was approximated by a constant, we assume after ref 22 the form g[ϕ(r)] = g2ϕ(r)2 + g0 with g2 = 4.01 − g0 and g0 = −3. In the mean-ﬁeld approximation the stable or metastable phases of the system correspond to the minimum of the functional (2). In order to minimize the functional, we discretize the ﬁeld ϕ(r) on the cubic lattice. The discretization and minimization procedures are described in detail in ref 22 (see also Supporting Information). After discretization, the problem of minimization of the functional is converted to the problem of minimization of a function of many variables, where the variables are the values of the ﬁeld ϕ(r) at the lattice points. We use the conjugate gradient method to minimize the function numerically.22,28,29 The Computational Method. In order to determine the structure of a given facet, we assume that ϕ(r) is periodic in the directions parallel to it while in the perpendicular direction the cubic and the isotropic phases are present at the two sides of the facet. We chose the coordinate frame with x and y directions parallel and z direction normal to the facet. Periodicity in x and y directions and the assumption that at large enough distance from the facet the bulk phases are not disturbed allow to obtain the structure of the near-surface layer of the cubic phase by translation in the x and y directions of the elementary computational cuboidal cell.

⎛ 2π ⎞ ⎛ 2π ⎞ ⎛ 2π ⎞ ⎛ 2π ⎞ cos⎜ x3⎟ − sin⎜ x1⎟ sin⎜ x 2⎟ sin⎜ x3⎟ ⎝L ⎠ ⎝L ⎠ ⎝L ⎠ ⎝L ⎠

(3)

where the coordinate frame is chosen such that xi are parallel to the edges of the cubic unit cell of the bulk phase. The linear size L of the periodic cubic element described by the nodal approximation 3 is taken as the size of the unit cell of the bulk bicontinuous cubic diamond phase, which is known from previous calculations.22 Such a cubic element of size L is shown in Figure 3b. We discretize the ﬁeld ϕ(r) in such a way that that

Figure 3. Computational cells for the facets: (a) (111) √6/2L × √2/ 2L × √3L, (b) (100) L × L × L, and (c) (110) √2/2L × L × √2/ 2L. Green and yellow colors show diﬀerent sides of the surface ϕ(r) = 0.

we have 65 lattice points on the length L. In the case of the calculations performed for (100) facets we use the lattice with 653 points per the cubic element (Figure 3b). Thus, for the computational cell of thickness 4L we use more than 1 million lattice points. Such a degree of discretization is more than enough to obtain the detailed structure of the facets. The initial conﬁgurations for all cuboids used to determine the structure of the facets perpendicular to the directions [111], [100], and [110] are shown in Figures 3a,b,c, respectively. The size of the cuboids in x and y directions is the period of the cubic phase in the corresponding direction. This size is kept constant. In z direction we consider a range of thicknesses of the cuboid, Zmin < Z < Zmax. We chose Zmax = 8Zmin. The size Zmin of the smallest cuboid in the z direction is equal to the period of the cubic phase in this direction. Z assumes the values which are multiples of the number of grid points times the distance between the grid points. For the facets (111) the x, y, z axis in the cuboid should be identiﬁed with [1̅01], [1̅21̅], and [111] directions, respectively. Thus, in the z direction the period for the (100), (110), and (111) is L, √2/2L, and √3L, respectively. The size of the cuboid, for calculating the (100) facets, in x and y direction is equal to L, and the size in z direction (normal to the facet (100)) is varied from L to 8L. The x, y, z axis in the cuboid should be identiﬁed with [100], [010], and [001] directions, respectively. The size of the cuboid, for calculating (110) facets, in x and y direction is equal to √2L and L, respectively. The size in z direction (normal to the facet (110)) is varied from √2/2L to 8√2/2L. The x, y, z axis in the cuboid should be identiﬁed with [1̅10], [001], and [110] directions, respectively. The size of the cuboid, for calculating (111) facets, in x and y direction is equal to √2/2L and √6/2L, respectively, while the

Figure 2. Cross section of the computational cuboidal cell. Z is the thickness of the cell in z direction. The sizes of the cell in x and y directions depend on the orientation of the facet and are shown in Figure 3. Periodic boundary conditions are imposed on the dashed lines. At the thin solid line ϕ(r) has the form obtained for the bulk phase. At the thick solid line ϕ(r) = 1, indicating the water-rich phase. l is the distance of the interface from the face of the computational cuboidal cell with ϕ(r) = 1.

The size of the cuboid in x and y directions is determined by the value of the unit-cell length of the bulk cubic phase and the orientation of a given facet. The sizes of the computational cells are diﬀerent for each facet due to diﬀerent symmetries in each case. We apply periodic boundary conditions in x and y directions and ﬁxed boundary condition in z direction, where the ﬁeld ϕ on one side of the cuboid is composed of the bulk cubic phase and on the other side it is ϕ = ±1 as in the isotropic phase. The facet is formed at the boundary with the isotropic phase, near the face of the cuboid with the boundary condition ϕ = ±1. We use the nodal approximation (eq 3) to triply periodic bicontinuous phases to build the initial conﬁguration for the ﬁeld ϕ(r) in the cuboids: 490

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

size in z direction (normal to the facet (111)) is varied from √3L to 8√8L.

subsequent facets formed at diﬀerent thickness of the bicontinuous phase are the same and equal to √3/6L. The formation of a new facet is related to the change of the topology of the growing nanoparticle or the monocrystal. The open channels at the (111) facets form a triangular lattice. The surface of the facet is approximately ﬂat. Such a unique structure of the (111) facets may explain their exceptional stability. The facets shown in Figure 4 are obtained for diﬀerent sizes of the cuboids (reﬂecting the structures of diﬀerent topology) for which the functional (2) has a minimum with respect to the thickness of the cubic phase in z direction. The change of the topology is monitored by the calculations of the genus of the surface ϕ(r) = 0 contained in the computational cell. The genus is obtained by calculating the Euler characteristics of the surface ϕ(r) = 030−36 (see Supporting Information for details). For the ﬁxed topology (the same genus), we obtain conﬁgurations for the (111) facets for which the free energy is optimized with respect to the thickness of the cubic phase in z direction. It means that when the thickness is decreased or increased from the optimal value, the free energy increases. In Figure 5, we plot the values of the free energy for the (111) facets as a function of the thickness of the cuboid F(Z).

3. RESULTS The functional (2) is minimized with respect to ϕ(r) with the imposed boundary conditions and for a given Z, where Z is the size of the computational cell in z direction. This way a function of Z, F(Z), equal to the minimum of the functional (2) for a given Z is obtained for the range of Zmin < Z < Zmax. F(Z) has local minima for Z = Zn with ﬁxed distance between them ΔZ = Zn+1 − Zn. ΔZ depends on the orientation of the facet. Each minimum corresponds to a diﬀerent topology of the layer of the cubic phase. F(Z) is the free energy under the constraint of ﬁxed thickness Z of the computational cell. When the constraints are released, the free energy assumes a minimum. We therefore identify the structure of the facet for a given topology with the structure obtained for Z = Zn. The corresponding surface describing the shape of the bilayer is given by ϕZn(r). Structure of the Facets. According to the experimental observations17 for Pn3̅m cubic bicontinuous phases, the most stable are the (111) facets. We calculated the structure of the facets perpendicular to three major directions ([111], [100], [110]) by minimizing the functional (2) subject to appropriate boundary conditions. Our goal was to examine the structure and the stability of the facets created at the interface between a monocrystal or a nanoparticle of the lyotropic liquid crystal phase surrounded by the isotropic phase. Facets Orthogonal to [111] Direction. Within the period of the cuboid (see Figure 3b) which is √3L along z axis, the facets can be formed at three diﬀerent positions when the channels of the bicontinuous phase are closed at one side of the surface composed of amphiphilic molecules (see Figures 4a,b,c) and at three other positions when the channels of the bicontinuous phase are closed on the other side of this surface (see Figures 4d,e,f). The distances between the positions of

Figure 5. (a) The Landau−Brazovskii free energy per unit volume as a function of the thickness of the cuboid (Z). (b) The Helfrich free energy per surface area of the plane parallel to the facet as a function of the thickness of the cuboid (Z). The distance on horizontal axis is given in units √3L, which is the period of the cuboid in z direction. The circles and the squares denote the conﬁgurations with the open channels on one or the other side of the surface ϕ(r) = 0.

We also show the Helfrich free energy calculated for ϕ(r) = 0 for the conﬁgurations obtained by minimization of the functional (2). It is interesting to note that the positions of the minima are approximately the same for the calculations performed for the functional (2) and the functional (1). Thus, we can speculate that the shapes of the facets obtained by direct minimization of the functional (1) would be very similar to the shapes obtained by direct minimization of the functional (2). It has to be noted that minimization of the functional (1) is much more diﬃcult since the parametrization of the surface of a cubic phase is practically impossible. Facets Orthogonal to [100] Direction. The (100) facets can be formed at four diﬀerent positions within the period of the cuboid L in z direction. The subsequent facets in the growing crystal are separated by the distance L/4. When a new facet is formed, then the topology is changed. The shapes of the

Figure 4. The (111) facets formed at diﬀerent thickness of the bicontinuous phase. The facets are formed when the thickness of the bicontinuous phase is increased by √3/6L. Left and right panels show the facets with closed channel at one of the two sides of the surface ϕ(r) = 0. The surface of the ﬁrst facet is bounded by the dashed line. The 3D view of the facets is shown in movies 1 and 2 of the Supporting Information. 491

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

facets for the thickness of the cubic phase in the range from z to z + L are presented in Figure 6. Unlike in the case of (111)

Figure 7. Two types of the (100) facets. Left and right panels show the facets formed when the bicontinuous phase is deformed more and less by the creation of the facet. In the second row, the conﬁgurations from the ﬁrst row are presented viewed from [100] direction. In the third row, the conﬁgurations from the ﬁrst row are presented viewed from [110] direction. The 3D view of the facets is shown in movie 5 of the Supporting Information.

ﬂat with the open channels forming a square lattice of holes as presented in Figure 7. The structures of (100) facets were studied in a lattice model.20,21 Only the structure with the bulges along the diagonal of the cubic cell was obtained in those calculations. This is because in the lattice model only a few lattice points form a cubic cell. In the continuous model, the order parameter ﬁeld is discretized on a large grid of points. Thus, the results of calculations can describe the structure of the facets more accurately. Facets Orthogonal to [110] Direction. In the case of the (110) facet, two conﬁgurations with diﬀerent topology can be distinguished within the period of the cuboid along the z axis. In Figure 8 we show the conﬁgurations with the lowest energy for the set of conﬁguration with the same topology. The (110) facets are formed when the thickness of the bicontinuous phase increases by √2/4L. The open channels of (110) facets are

Figure 6. The (100) facets formed at diﬀerent thickness of the bicontinuous phase. The facets are formed when the thickness of the bicontinuous phase is increased by 1/4L. Left and right panels show the facets with closed channel at one of the two sides of the surface ϕ(r) = 0. The surface of the ﬁrst facet is bounded by the dashed line. The 3D view of the facets is shown in movies 3 and 4 of the Supporting Information.

facets, at the same thickness of the bicontinuous phase, two diﬀerent facets may be formed when the channels are closed on one or the other side of the surface ϕ(r) = 0. These facets are structurally and energetically the same. The conﬁguration in the left and right columns are obtained when the channels are closed on green side or yellow side of the surface ϕ(r) = 0. At each row the conﬁgurations obtained for the same thickness of the cubic phase are presented. It is interesting to note that for (100) facets we can obtain two structures of the facets for a given ﬁxed topology. They are stable and have similar energies. The shape of the facets are shown in Figure 7. Amphiphilic molecules in bulk bicontinuous phase form a surface which is identical with a triply periodic minimal surface. Such conﬁguration has the lowest energy. At the boundary with the isotropic phase, the triply periodic surface has to be deformed in order to avoid conﬁgurations with free edges exposed to the isotropic phase. The interior of the crystal of the bicontinuous phase can be deformed, and this deformation depends on the structure at the boundary. If the structure of the facet at the boundary is such that its energy is optimized, then the bicontinuous phase is deformed more away from the boundary. However, it is also possible to avoid large deformations of the bicontinuous phase. In such a case the energy of the facets is not optimized. This leads to two kinds of facets which are presented in Figure 7. The ﬁrst one of those facet structures is formed when the channels, which are closed, form cylindrical bulges directed along the diagonal of the computational cell. The second conﬁguration is appropriately

Figure 8. The (110) facets formed at diﬀerent thickness of the bicontinuous phase. The facets are formed when the thickness of the bicontinuous phase is increased by √2/4L. Left and right panels show the facets with closed channel at one of the two sides of the surface ϕ(r) = 0. The surface of the ﬁrst facet is bounded by the dashed line. The 3D view of the facets is shown in movies 6 and 7 of the Supporting Information. 492

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

when the energy is calculated from the functional (1) where only the shape of the surface ϕ(r) = 0 is considered. Thus, we can safely restrict the analysis of the data obtained from minimization of the functional (2) to the surface ϕ(r) = 0. In an ideal situation the mean curvature of a triply periodic minimal surface should be zero at every point. In practice, in numerical calculations the mean curvature is very close to zero. The formation of the facets deforms the triply periodic minimal surface. This deformation and thus deviation of the mean curvature from the optimal value are the largest in the vicinity of the facet. When analyzing the values of the local mean curvature on a surface ϕ(r) = 0, we observed that the deformation of the triply periodic minimal surface due to formation of the facets propagates inside the cubic phase up to the distance of one, two unit cell length L. (The mean curvature was computed from the ﬁeld ϕ(r); see Supporting Information for details.) This suggests that the cubic phase inside a monocrystal (cubosome) is signiﬁcantly deformed only near its boundary with an isotropic phase. We can try to deﬁne a speciﬁc “surface (interfacial) energy” associated with this deformation. The deformation should be diﬀerent for diﬀerent facets since the cubic phase is anisotropic. We can suspect that the stability of diﬀerent facets may be related to diﬀerent surface energies for diﬀerent facets. We have estimated and compared the energies of formation of diﬀerent facets by calculating the bending energy (1) for the same size of the cuboids in z direction and dividing it by the surface area of the computational cell in the x−y plane. Such energy was the smallest for (111) facets and the biggest for (110) facets. This is in agreement with the results of the experiments in which (111) facets are the most stable. Moreover, the diﬀerence in energy between (111) and (100) facets is larger than the diﬀerence in energy between (100) and (110) facets. The better stability of more ﬂat facets may be explained by considering the mean curvatures of the surface ϕ(r) = 0. Both a plane and a triply periodic minimal surface have zero mean curvature at every point. Thus, in order to minimize the functional (1), it would be the best if the surface ϕ(r) = 0 were built mainly of planar and triply periodic minimal surfaces. Unfortunately “gluing” these two surfaces results in their deformations. From our calculations it follows that these deformations are the largest for (110) facets and the smallest for (111) facets.

arranged in a triangular lattice for the optimal conﬁgurations. This is very similar to the conﬁgurations obtained for (111) facets. The diﬀerence between these two type of facets is manifested when the thickness of the cubic phase is not optimal. In the case of (111) facets the open channels are still arranged in a triangular lattice, but for (110) facets this triangular order is no longer present. In Figure 9, the right

Figure 9. Two types of the (110) facets. Left and right panels show zigzag and ﬂat facets, respectively. In the second row, the conﬁgurations from the ﬁrst row are presented viewed from direction parallel to the x axis. In the third row, the conﬁgurations from the ﬁrst row are presented viewed from direction parallel to the z axis. The 3D view of the facets is shown in movie 8 of the Supporting Information.

column shows the conﬁguration for (110) facet with the open channels arranged in a triangular lattice and the left column shows the conﬁgurations without triangular order. The conﬁgurations with triangular arrangements of the open channels are more ﬂat then the one without the triangular order. However, they are less ﬂat than the conﬁgurations obtained for (111) facets. Only one of these conﬁgurations is stable for a given thickness of the facet. For a ﬁxed topology the more stable conﬁguration is the one with more ﬂat facets as shown in Figure 9. In the case of (111) and (100) facets the channels are parallel and perpendicular to the [111] and [100] direction, respectively. In the case of (110) facets the channel are at an angle to the [110] direction. The formation of a ﬂat facet should be the easiest for the [111] direction since it is enough to connect the channels with a approximately planar surface and the triply periodic surface can be deformed at the connection. The formation of (100) facet should be more diﬃcult since the channels should be closed by a semicylindrical surface. In the case of (110) facet the adjacent channels are directed at a certain angle. Therefore, the formation of a ﬂat surface will require larger deformation of the triply periodic surface near the facet, as shown in Figure 9. Stability for Diﬀerent Directions. We have analyzed the stability of the facets by calculating also the bending energy Fb per surface area for the surface ϕ(r) = 0 contained inside the computational cell. The conﬁgurations with the lowest energy are the same both when the energy is calculated from the functional (2) where the ﬁeld ϕ(r) is taken into account and

4. EXPERIMENTAL OBSERVATION OF CUBOSOMES It is impossible to determine the structure of the facets of monocrystals of lyotropic cubic liquid crystals by optical microscopy. We decided to obtain dispersion of nanoparticles of lyotropic cubic liquid crystals experimentally and to examine their structure under cryo-TEM. We have prepared the cubosomes of phytantriol using a method analogous to the method developed for cubosomes made of glycerol monoolein.37 To prepare cubosomes, we mixed some amount of phytantriol with water and a stabilizer Poloxamer-407. The standard method of preparation of the cubosomes gives the particles of Pn3̅m symmetry. We mixed some amount of phytantriol with the stabilizer (according to ratio in the publication) and water. Next, the mixture was ultrasonicated within 0 or 15 min (depending on the method). The cubosomes were cryo-ﬁxed on day of their preparation and analyzed on the second day of cryo-ﬁxation. The role of the stabilizer is crucial in obtaining stable nanoparticles. We have 493

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

monocrystal. We have also checked if the formation of the facets inﬂuences the periodicity of the bicontinuous phase. We have changed the size of the unit cell L decreasing it and increasing. We have not seen any decrease in energy for increased or decreased values of L. We have estimated the surface energy associated with the formation of the (111), (100), and (110) facets. On the basis of these calculations, we can predict that the most stable facet is the one which is ﬁrst formed in the experiments,17 namely (111).

attempted to produce the nanoparticles without the stabilizer, but the nanoparticles were unstable and were very quickly stuck together. We can speculate that the stabilizer is attached to the bilayer at the walls of the cubosomes, but it does not inﬂuence signiﬁcantly its internal structure even in often encountered cases where a vesicle is attached to a wall of a cubosome. So far cryo-TEM is the best technique to study the structure of small soft objects of the order of 100 nm. From images obtained from cryo-TEM it is possible to infer the information about the internal structure of the nanoparticles and their shape. The cubosomes have usually polyhedral shape as shown in Figure 10. Unfortunately, the structure of the faces of the

■

ASSOCIATED CONTENT

S Supporting Information *

Details of the numerical calculations and movies showing 3D views of the facets. This material is available free of charge via the Internet at http://pubs.acs.org.

■

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected] (W.T.G.). Notes

The authors declare no competing ﬁnancial interest.

■

ACKNOWLEDGMENTS W. Gózd́ ź acknowledges the support from NCN Grant 2012/ 05/B/ST3/03302. The work of L. Latypova was realized within the International PhD Projects Programme of the Foundation for Polish Science, coﬁnanced from European Regional Development Fund within Innovative Economy Operational Programme “Grants for innovation”. The authors thank Alina Ciach for helpful discussions. We thank Jeril Degrouard for his help in performing cryo-TEM experiments.

■

REFERENCES

(1) Ciach, A.; Pȩkalski, J.; Gózd́ ź, W. T. Origin of Similarity of Phase Diagrams in Amphiphilic and Colloidal Systems with Competing Interactions. Soft Matter 2013, 9, 6301−6308. (2) Seul, M.; Andelman, D. Domain Shapes and Patterns: The Phenomenology of Modulated Phases. Science 1995, 267, 476−483. (3) Luzzati, V.; Tardieu, A.; Gulik-Krzywicki, T.; Rivas, E.; ReissHusson, F. Structure of the Cubic Phases of the Lipid-Water Systems. Nature 1968, 220, 485−488. (4) Scriven, L. E. Equilibrium Bicontinuous Structure. Nature 1976, 263, 123−125. (5) Hajduk, D. A.; Harper, P. E.; Gruner, S. M.; Honeker, C. C.; Kim, G.; Thomas, E. L.; Fetters, L. J. The Gyroid: A New Equilibrium Morfology in Weakly Segregated Diblock Copolymers. Macromolecules 1994, 27, 4063−4075. (6) Ciach, A.; Gózd́ ź, W. T. 7 Nonelectrolyte Solutions Exhibiting Structure on the Nanoscale. Annu. Rep., Sect. C 2001, 97, 269−314. (7) Almsherqi, Z. A.; Kohlwein, S. D.; Deng, Y. Cubic Membranes: A Legend beyond the Flatland of Cell Membrane Organization. J. Cell Biol. 2006, 173, 839−844. (8) Helfrich, W. Elastic Properties of Lipid Bilayers: Theory and Possible Experiments. Z. Naturforsch., A 1973, 28, 693. (9) Haluska, C. K.; Gózd́ ź, W. T.; Döbereiner, H.-G.; Förster, S.; Gompper, G. Giant Hexagonal Superstructures in Diblock-Copolymer Membranes. Phys. Rev. Lett. 2002, 89, 238302. (10) Gózd́ ź, W. T. Spontaneous Curvature Induced Shape Transformation of Tubular Polymersomes. Langmuir 2004, 20, 7385−7391. (11) Gózd́ ź, W. T. Influence of Spontaneous Curvature and Microtubules on the Conformations of Lipid Vesicles. J. Phys. Chem. B 2005, 109, 21145−21149.

Figure 10. Images of the cubosomes obtained by cryo-TEM on the ﬁrst day after preparation defocus 4000 nm. The size of the cubosomes is of the order of 150 nm.

cubosomes can be inferred only indirectly from the cryo-TEM images. Nevertheless, if we assume that cubosomes are attached to the carbon grid on which the samples are prepared so that the surface of the grid touches the surface of the facet we can deduce by looking at the periodic structure of the image which facets are mainly formed. The images obtained by scattering the beam of electrons from the cubosomes (see Figure 10) are characterized by periodic patterns. We can clearly observe triangular and square lattice structures. This would suggest that the faces of cubosomes have the structure similar to the structure calculated for (111) and (100) facets.

5. CONCLUSIONS We have used Landau−Brazovskii functional to determine the structure and stability of the facets of monocrystals of the lyotropic cubic bicontinuous phase Pn3̅m. In the theoretical model presented here, the calculations are performed for inﬁnitely large facets built of identical elements. We have determined the structure of the (111), (100), and (110) facets for the cubic phase of Pn3̅m symmetry. We have predicted the possible shape of the surface composed of amphiphilic molecules at the facets in detail. Our calculations suggest that the cubic phase is deformed mainly near the faces of the 494

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495

Langmuir

Article

(12) Pierański, P.; Even, C.; Rohe, D.; Sittler, L.; Bouchih, M.; Ginestet, N.; Popa-Nita, S.; Plötzing, T.; Grenier, J. New Faceting Phenomena in Lyotropic Liquid Crystals. Mol. Cryst. Liq. Cryst. 2005, 434, 235/[563]−249/[577]. (13) Gustafsson, J.; Ljusberg-Wahren, H.; Almgren, M.; Larsson, K. Cubic Lipid-Water Phase Dispersed into Submicron Particles. Langmuir 1996, 12, 4611−4613. (14) Gustafsson, J.; Ljusberg-Wahren, H.; Almgren, M.; Larsson, K. Submicron Particles of Reversed Lipid Phases in Water Stabilized by a Nonionic Amphiphilic Polymer. Langmuir 1997, 13, 6964−6971. (15) Barauskas, J.; Johnsson, M.; Joabsson, F.; Tiberg, F. Cubic Phase Nanoparticles (Cubosome): Principles for Controlling Size, Structure, and Stability. Langmuir 2005, 21, 2569−2577. (16) Spicer, P. T. Progress in Liquid Crystalline Dispersions: Cubosomes. Curr. Opin. Colloid Interface Sci. 2005, 10, 274−279. (17) Latypova, L.; Gózd́ ź, W. T.; Pierański, P. Symmetry, Topology and Faceting in Bicontinuous Lyotropic Crystals. Eur. Phys. J. E 2013, 36, 88. (18) Schnering, H.; Nesper, R. Nodal Surfaces of Fourier Series: Fundamental Invariants of Structured Matter. Z. Phys. B: Condens. Matter 1991, 83, 407−412. (19) Babin, V.; Ciach, A. Double-Diamond Phase in Amphiphilic Systems Confined between Parallel Walls. J. Chem. Phys. 2001, 115, 2786−2793. (20) Babin, V.; Ciach, A. Response of the Bicontinuous Cubic D Phase in Amphiphilic Systems to Compression or Expansion. J. Chem. Phys. 2003, 119, 6217−6231. (21) Ciach, A.; Høye, J.; Stell, G. Bicontinuous Phase in a Lattice Model for Surfactant Mixtures. J. Chem. Phys. 1991, 95, 5300. (22) Gózd́ ź, W. T.; Hol̷yst, R. Triply Periodic Surfaces and Multiply Continuous Structures from the Landau Model of Microemulsions. Phys. Rev. E 1996, 54, 5012−5027. (23) Gózd́ ź, W. T.; Hol̷yst, R. High Genus Periodic Gyroid Surfaces of Nonpositive Gaussian Curvature. Phys. Rev. Lett. 1996, 76, 2726− 2729. (24) Gompper, G.; Schick, M. Self-Assembling Amphiphilic Systems, 1st ed.; Academic Press: London, 1994; Vol. 16. (25) Leibler, L. Theory of Microphase Separation in Block Copolymers. Macromolecules 1980, 13, 1602. (26) Fredrickson, G. H.; Helfand, E. Fluctuation Effects in the Theory of Microphase Separation in Block Copolymers. J. Chem. Phys. 1987, 87, 697. (27) Brazovskii, S. A. Phase Transition of an Isotropic System to a Nonuniform State. Sov. Phys. JETP 1975, 41, 8. (28) Press, W. H.; Flannery, B. P.; Teukolsky, S. A.; Vetterling, W. T. Numerical Recipes; Cambridge University Press: New York, 1990. (29) Lorensen, W. E.; Cline, H. E. Marching Cubes: A High Resolution 3D Surface Construction Algorithm. Comput. Graphics 1987, 21, 163−169. (30) Hoffman, D. A. Some Basic Facts, Old and New, About Triply Periodic Embedded Minimal Surfaces. Colloq. Phys. 1990, 51 (C7), 197−208. (31) Anderson, D. M.; Davis, H. T.; Scriven, L. E.; Nitsche, J. C. C. Periodic Surfaces of Prescribed Mean Curvatures. Adv. Chem. Phys. 1990, 77, 337−396. (32) Weatherburn, C., Ed.; Diﬀerential Geometry of Three Dimensions; Cambridge University Press: New York, 1930; Vol. II. (33) Mackay, A. L.; Klimowski, J. Towards a Grammar of Inorganic Structure. Comput. Math. Appl. 1986, 12B, 803−824. (34) Gandy, P. J.; Bardhan, S.; Mackay, A. L.; Klinowski, J. Nodal Surface Approximations to the P,G,D and I-WP Triply Periodic Minimal Surfaces. Chem. Phys. Lett. 2001, 336, 187−195. (35) Barnes, I. S.; Hyde, S. T.; Ninham, B. W. The Caesium Chloride Zero Potential Surface Is Not the Schwarz P-Surface. Colloq. Phys. 1990, 51 (C7), 19−24. (36) Spivak, M. A Comprehensive Introduction to Diﬀerential Geometry; Publish or Perish: Berkley, CA, 1979; Vol. III.

(37) Spicer, P. T.; Hayden, K. L.; Lynch, M. L.; Ofori-Boateng, A.; Burns, J. L. Novel Process for Producing Cubic Liquid Crystalline Nanoparticles (Cubosomes). Langmuir 2001, 17, 5748−5756.

495

dx.doi.org/10.1021/la4040744 | Langmuir 2014, 30, 488−495